Photobactericidal Porphyrin-Cellulose Nanocrystals: Synthesis, Characterization, and Antimicrobial Properties Elke Feese,† Hasan Sadeghifar,‡,# Hanna S. Gracz,§ Dimitris S. Argyropoulos,†,‡,|| and Reza A. Ghiladi*,† Departments of Chemistry, ‡Forest Biomaterials, and §Molecular and Structural Biochemistry, North Carolina State University, Raleigh, North Carolina, United States Department of Chemistry, University of Helsinki, Helsinki, Finland # Department of Wood and Paper Science, Islamic Azad University, Chalous, Iran
bS Supporting Information ABSTRACT: Adherence and survival of pathogenic bacteria on surfaces leading to concomitant transmission to new hosts signiﬁcantly contributes to the proliferation of pathogens, which in turn considerably increases the threat to human health, particularly by antibiotic-resistant bacteria. Consequently, more research into eﬀective surface disinfection and alternative materials (fabrics, plastics, or coatings) with antimicrobial and other bioactive characteristics is desirable. This report describes the synthesis and characterization of cellulose nanocrystals that were surface-modiﬁed with a cationic porphyrin. The porphyrin was appended onto the cellulose surface via the Cu(I)-catalyzed HuisgenMeldalSharpless 1,3-dipolar cycloaddition having occurred between azide groups on the cellulosic surface and porphyrinic alkynes. The resulting, generally insoluble, crystalline material, CNC-Por (5), was characterized by infrared and diﬀusion 1H NMR spectroscopies, gel permeation chromatography, and thermogravimetric analysis. Although only suspended, and not dissolved, in an aqueous system, CNC-Por (5) showed excellent eﬃcacy toward the photodynamic inactivation of Mycobacterium smegmatis and Staphylococcus aureus, albeit only slight activity against Escherichia coli. The synthesis, properties, and activity of CNC-Por (5) described herein serve as a benchmark toward our overall objectives of developing novel, potent, bioactive, photobactericidal materials that are eﬀective against a range of bacteria, with potential utilization in the health care and food preparation industries.
ospital acquired infections, in particular, highlight the issue of adherence and survival of bacteria on surfaces leading to an increase in the proliferation and transmission of bacteria. Speciﬁcally, antibiotic-resistant bacteria are a rising threat to human health. According to the Centers of Disease Control and Prevention, about 1.7 million healthcare associated infections cause upward of 99000 deaths annually in the United States.1 A total of 510% of all hospitalized patients are adversely aﬀected, which in turn is adding about $3045 billion to health care costs annually.2 Food processing/packaging, food service, and wastewater treatment industries, as well as personal households, are also areas of concern and can contribute to the spread of disease through contaminated or improperly disinfected surfaces. Consequently, more research into eﬀective surface disinfection and alternative materials (fabrics, plastics, or coatings) with antimicrobial properties is needed. Several classes of antimicrobial agents are currently being investigated or are commercially available, among which are polymeric compounds containing quarternary ammonium,37 pyridinium8,9 or phosphonium salts,5,10 N-halamines,11,12 biguanides,13 antibiotics,14 heavy metals such as Ag,1416 and phenol derivatives.14 Disadvantages of currently available materials are the loss of antimicrobial activity r 2011 American Chemical Society
by leaching of the biocide in noncovalent systems, consumption of the germicidal ability, environmentally hazardous agents, or dependency on direct contact of the antimicrobial entity with the microorganism. Thus, there is an urgent need for the development of novel materials with the potential capability of rapid, eﬃcient, and low-cost sterilization of a range of bacteria. During the past few decades, photodynamic inactivation (PDI) has garnered the attention of many researchers as an alternative technique for eradicating microorganisms. Therefore, we see great potential in the development of photobactericidal materials that could satisfy many desired characteristics while overcoming some of the shortcomings of currently available antimicrobial materials. PDI employs a localized, light-activated photosensitizer (PS) that generates cytotoxic species, particularly singlet oxygen, upon illumination with visible light. Singlet oxygen, as opposed to some common disinfectants such as chlorine and hypochlorite, can be regarded as an environmentally benign germicide (short lifetime of 106 s in water17 and Received: May 27, 2011 Revised: August 3, 2011 Published: August 12, 2011 3528
dx.doi.org/10.1021/bm200718s | Biomacromolecules 2011, 12, 3528–3539
Scheme 1. Synthesis of Cellulose Nanocrystal-Porphyrin Conjugate CNC-Por (5)
reverting back to harmless ground state oxygen if unreacted). Singlet oxygen is known to be able to diﬀuse over signiﬁcant distances, as long as 100200 nm in water and about 1 mm in air.18 Bezman et al. were the ﬁrst to demonstrate this by photodynamic inactivation of E. coli with Rose Bengal immobilized on polystyrene beads.19 Dahl et al. demonstrated the successful photodynamic inactivation of Salmonella lyphimurium and E. coli by the ﬂow of singlet oxygen through a 0.65 mm air gap between the microbes and a photosensitizer.20 The feasibility of the concept of a “photobactericidal surface” is further supported by studies showing that the photosensitizers retain their ability to reduce a bacterial cell count when adsorbed, codissolved and casted, as well as covalently bound, to nanoparticles,21,22 polymers,23,24 ﬁlms,2527 or membranes.28 Of particular interest for our work is a series of studies by Krausz and co-workers who have investigated the incorporation of selected porphyrin photosensitizers into cellulose esteriﬁed plastic ﬁlms and demonstrated the photobactericidal activity of such ﬁlms.26,27,29 Cellulose is Earth’s most abundant natural biopolymer, consisting of high molecular weight β-1,4-linked anhydro-D-glucose polymer chains, and therefore, in our eyes, an excellent starting material for developing new, more sustainable materials from renewable resources.30,31 Distortions in the hydrogen bonding of the tightly cross-linked chain packing causes amorphous regions within the otherwise crystalline microﬁbrils. Acidic hydrolysis of these defects results in rod-shaped cellulose nanocrystals [CNC (1), Figure SD1] with high mechanical strength and etched, chemically modiﬁable, molecular surface patterns.3133 For example, these nanomaterials are rigid rods, with embedded chirality, and a unique etched nanopattern composed of primary hydroxymethyl groups on their surface that may readily be further functionalized for the purposes of anchoring a variety of molecules onto them.33 Furthermore, these nanomaterials, being of a carbohydrate nature, are of inherent compatibility with
biological tissue and, therefore, of unique utility with respect to their bioavailability, biocompatibility, and biodegradability considerations. Consequently, the focus of the present report is the surface modiﬁcation of cellulose nanocrystals CNC (1) with the cationic porphyrin (Por) 4, yielding the conjugate CNC-Por (5) (Scheme 1). The advantages of a covalent attachment of the porphyrin to the surface of the cellulose nanocrystals potentially include conferring longer lasting or permanent antimicrobial properties to the cellulose (improved durability), minimizing the leaching of the biocidal agent into the surrounding environment, and prevention of porphyrin aggregation. The covalent attachment of 4 to 1 was achieved via the Cu(I)catalyzed HuisgenMeldalSharpless 1,3-dipolar cylcoaddition (hereafter referred to as an example of a “Click reaction”) between an azide on the CNC surface and the alkyne-containing porphyrin.34,35 To the best of our knowledge, this work is among the ﬁrst attempts to covalently append cationic porphyrins to the surface of cellulose nanocrystals. The physicochemical characteristics of CNC-Por (5) were investigated using a combination of spectroscopic and chemical analyses, thereby demonstrating the covalent linkage between the two moieties, while its photobactericidal characteristics were also investigated. As will be shown, CNC-Por (5) was highly eﬃcient in mediating the photodynamic inactivation of M. smegmatis and S. aureus, and did exhibit some activity against E. coli. The potential and the signiﬁcance of CNC-Por (5) in the context of cellulose-derived antimicrobial fabrics is highlighted by the fact that S. aureus has been found to be able to survive for weeks under dry conditions on cotton fabrics used in hospital environments.36,37 As such, we see possibilities for the incorporation of photosensitizer-modiﬁed-cellulose nanocrystals into paper, fabrics and plastics, thereby creating novel, biodegradable, photobactericidal materials from renewable sources 3529
dx.doi.org/10.1021/bm200718s |Biomacromolecules 2011, 12, 3528–3539
Biomacromolecules that may be capable of sterilizing a range of bacteria with high eﬃcacy, rapidly, and at minimal cost.
’ MATERIALS AND METHODS Materials. Buffer salts were purchased from Fisher Scientific, Middlebrook 7H9 agar and 7H10 broth from BD Difco, LB broth Miller from EMD Chemicals and Tryptic Soy Broth from Teknova. Unless otherwise specified, all other chemicals were obtained from commercial sources in the highest purity available. Ultrapure water used for all media and buffers was provided by an Easypure II system (Barnstead). UVvisible absorption measurements were performed on a Varian Cary 50 Bio instrument or a Genesys 10 UV scanning spectrophotometer from Thermo Electron Corp for single wavelength measurements. All procedures were carried out under commonly practiced sterile techniques. A Perkin-Elmer Model 3110 atomic absorption spectrometer was used for the determination of the Zn ion content of 5. FT-IR (Fourier transform infrared) spectra were measured on a Thermo Nicolet NEXUS 670 FT-IR spectrophotometer. Spectra in the range of 4000650 cm1 were obtained with a resolution of 4 cm1 by accumulating 64 scans. Thermal decomposition temperatures were determined using a TA Instrument TGAQ500 ramping 10 °C/min under N2 purging. CNC samples were dried using a lyophilizing system from Labconco (Kansas City, Mo, USA). For Transmission Electron Microscopy (TEM), a suspension (0.01% w/v in water) of cellulose nanocrystals were deposited as drops on carbon-coated electron microscope grids, negatively stained with uranyl acetate, and allowed to dry. The grids were observed with a Philips 400T microscope operated at an accelerating voltage of 120 kV. Formation of Cellulose Nanocrystals, CNC (1). The cellulose nanocrystals employed in this study were formed by acidic hydrolysis as reported in the literature with only minor modification.33,38,39 Briefly, 2.0 g of cellulose pulp were obtained from Whatman #1 filter paper (98% α-cellulose, 80% crystallinity) and blended in a 10 Speed Osterizer Blender. Hydrolysis of the resulting pulp was achieved after 3 h at 100 °C using 100 mL of 2.5 M HBr and intermittent ultrasonication (5 min per hour, 50% power, Omni Ruptor 250 W ultrasonic homogenizer). After dilution with deionized water, the mixture was subjected to five washing/centrifugation cycles (5000g, 10 min, IEC Centra-CL3 Series) to remove excess acid and water-soluble fragments. Once pH 45 was reached, the fine cellulose particles started to disperse into the aqueous supernatant. The polydisperse cellulose contained in the turbid supernatant was collected and subjected to centrifugation at 15,000g for 60 min in a Sorvall Superspeed centrifuge to remove ultrafine particles. The sediment containing the cellulose nanocrystals with an average length of 100400 nm was dried using a lyophilizing system, yielding 0.9 g CNC (1; 47% yield). Surface Tosylation of Cellulose Nanocrystals Yielding CNC-Tos (2). Surface-tosylated CNC was synthesized analogous to the method described by Rahn et al.40 0.5 g of CNC (1; 4 mmol glucosyl units) was suspended in pyridine (10 mL) and the mixture was cooled to 10 °C. Tosyl chloride (0.9 g, 5 mmol) was then added, and the reaction mixture was stirred for 2 days at room temperature. Addition of 100 mL of ethanol to the reaction mixture resulted in a precipitate that was collected by filtration. The product was washed with ethanol (50 mL) and deionized water (50 mL) five times each and freeze-dried, yielding 0.585 g CNC-Tos (2). Surface Azide Bearing CNC-N3 (3). Synthesis of the azide surface-modified cellulose nanocrystals, CNC-N3 (3), was conducted according to literature procedures with some modifications.33,4143 A total of 400 mg CNC-Tos (2) was suspended in 20 mL of DMF (N,Ndimethylformamide), followed by careful addition of 400 mg sodium azide. The reaction mixture was stirred at 100 °C for 24 h. After precipitation through the addition of 50 mL of deionized water and
centrifugation, the product was washed five times with ethanol (50 mL) and five times with deionized water (50 mL). The resulting product was dialyzed against deionized water for 3 days and, consequently, freezedried to yield 330 mg CNC-N3 (3; 84%). The degree of substitution (DS) was calculated from the elemental analysis (C 41.06%, H 6.35%, O 48.84%, N 3.75%) DS = 0.14. Click Reaction of CNC-N3 (3) with Porphyrin (4). Conditions for the Cu(I)-catalyzed HuisgenMeldalSharpless 1,3-dipolar cycloaddition reaction were selected from the literature.33,35,42,44,45 A total of 400 mg of CNC-N3 (3) and 400 mg of porphyrin 4 were mixed in 30.0 mL of DMF (99.5% purity). A mixture of 30 mg CuBr2, 70 mg ascorbic acid, and 200 μL of triethylamine in 1 mL of DMF was then added, and the reaction mixture was stirred vigorously for 5 min at room temperature, followed by stirring at 60 °C for 36 h. The product was isolated by centrifugation and washed three times with ethanol and three times with water (50 mL each time). For subsequent characterization and the photodynamic inactivation studies, the CNC-Por material was divided into ∼100 mg aliquots, and each aliquot was further washed to remove any unreacted porphyrin 4 (4 15 mL with DMF, 3 15 mL with 0.05 M acetic acid, 4 15 mL with water, and 3 15 mL with ethanol). After washing, the final product was isolated by 60 min centrifugation at 12000g and freeze-dried, yielding 480 mg of CNCPor (5) material. Acetylation of CNC-N3 (3) and CNC-Por (5). For the PFGSENMR (pulsed field gradient spin echo nuclear magnetic resonance) spectroscopic studies, samples of CNC-N3 (3) and CNC-Por (5) were acetylated to generate DMSO-soluble derivatives according to literature procedure with minor modification.4648 A total of 100 mg of the CNCderivative was dissolved in 3 g 1-allyl-3-methylimidazolium chloride (about 3% w/w) at 80 °C for 12 h. Acetic anhydride (315 μL; 5 mol/mol anhydrous glucose units) was added to the solution, and the mixture was stirred for 2 h at 80 °C. The product was precipitated by addition of 30 mL of deionized water and washed seven times with water. The CNC-derivative was obtained after freeze-drying and residual water was removed under high vacuum. Benzoylation of CNC-N3 (3) and CNC-Por (5). A total of 50 mg of either CNC-N3 (3) or CNC-Por (5) was dissolved in 1-allyl-3-methylimidazolium chloride (950 mg) in a 15 mL flask by first thoroughly dispersing the sample, followed by heating at 80 °C with magnetic stirring until the solution was transparent (about 4 h). Pyridine (330 μL, 3.7 mmol) was added, and the mixture was homogenized to form a uniform paste before being allowed to cool to room temperature. Benzoyl chloride (380 μL, 3.3 mmol) was then added in one portion, and the sample was subsequently stirred for 3 h at room temperature. The benzoylated product was precipitated by the addition of a 1:3 mixture of deionized water and EtOH with vigorous stirring for 5 min, after which the precipitate was collected by filtration using a medium porosity sintered glass funnel. The collected material was washed with EtOH and triturated with MeOH at room temperature for 18 h. The final product was collected by filtration and dried under vacuum to yield a green powder. Gel Permeation Chromatography. GPC analysis was carried out with a Waters model ALC/GPC 204 (Waters Associates, Milford, MA) and 510 pump equipped with a UV detector (210 nm). The analysis was conducted at 40 °C using THF as the eluent at a flow rate of 0.7 mL/min. A total of 200 μL of a 1 mg/mL solution of the analyte in THF was injected onto two Ultrastyragel columns (Styragel HR 1 and Styragel HR 5E, Waters) connected in series for analysis. Standard monodisperse polystyrenes (molecular weight ranges from 0.82 to 1860 kg/mol) were used for calibration. The number (Mn) and weight (Mw) average molecular weights were calculated using the Millenium 32 software.
Determination of Porphyrin Loading in CNC-Por (5) by Atomic Absorption Spectroscopy. Atomic absorption spectroscopy 3530
dx.doi.org/10.1021/bm200718s |Biomacromolecules 2011, 12, 3528–3539
Biomacromolecules was used to determine the concentration of Zn ions in samples of CNCPor (5), which is equivalent to the porphyrin loading if complete metalation of the porphyrin is assumed. About 10 mg of lyophilized CNC-Por (5) was suspended in 10 mL of 1 M HCl in a volumetric flask. The solution was heated to 60 °C for 2 h resulting in demetalation of the porphyrin. The zinc ion concentration was determined using the standard addition method: To each sample for the calibration curve (range of 0.010.1 mmol/L Zn(OAc)2 in 1 M HCl), 1 mL of the demetalated CNC-Por stock solution was added for a total volume of 10 mL. Under these conditions, the response of the atomic absorption instrument containing a Zn lamp operated at 10 mA was linear. The zinc ion concentration of the sample was calculated from the Y-intercept and the slope of the calibration curve. Typical porphyrin loadings were in the range of 0.16 ( 0.03 μmol porphyrin/mg of CNC-Por (5). Determination of the Zn content was done in triplicate for each batch of 5 synthesized.
Pulsed-Field-Gradient, SpinEcho NMR Spectroscopy.49,50 Modification of the glucoseOH groups by acetylation rendered the resulting CNC-Por compound sufficiently soluble in DMSO-d6 to conduct NMR spectroscopic studies. Spectra were obtained on a Bruker Avance 500 MHz spectrometer (1996) with an Oxford Narrow Bore Magnet (1989), Dell Host Workstation, and Red Hat Linux operation system with Topspin 2.1 software. The instrument was equipped with three-channel gradient control (GRASPIII), variable-temperature-, precooling-, temperature stabilization, as well as three frequency channels with waveform memory and amplitude shaping units. 1H NMR (proton nuclear magnetic resonance spectroscopy) diffusion measurements were conducted with a 5 mm triple axis gradient probe (ID5005EB, Nalorac Cryogenic Corp) equipped with actively shielded gradient coils. The gradient strength was calibrated using literature values for water diffusion in 1H2O/2H2O mixtures. The longitudinal eddy current (LED) pulse sequence was used in all diffusion experiments.51,52 A total of 10 gradient experiments were acquired for each data set. The gradient strength was adjusted linearly from 5.3 to 47.7 G/cm and applied in the y-direction, while all other delays were held constant. The gradient pulse interval Δ was 10 ms, the gradient duration δ 5 ms, with a recovery time of 6 ms. Acquisition temperature was 24.5 °C. The attenuation of the signal intensities derived from the peak height of each experiment was used to generate StejskalTanner plots to determine the diffusion coefficients. Diffusion coefficients were estimated by least-squares regression. Preparation of Photosensitizer Stock Solutions. Stock solutions (1 mM) of photosensitizers in filter-sterilized ultrapure water were prepared based on the porphyrin content determined by atomic absorption spectroscopy, in the case of CNC-Por (5), and stored in the dark at 80 °C. At the concentrations employed, turbidity of CNCPor (5) solutions was noted. Bacterial Strains and Growth Conditions. The bacterial strains Mycobacterium smegmatis mc2 155 (donated by Prof. William Jacobs, Albert Einstein College of Medicine, U.S.A.), Escherichia coli BL21(Dε3)pLysS (Strategene, U.S.A.) and Staphylococcus aureus 29213 (donated by Prof. Christian Melander, North Carolina State University, U.S.A.) were used in this study. M. smegmatis was grown in 5 mL cultures in Middlebrook 7H9 media with ADS (albumin dextrose saline) and 100 μg/mL cycloheximide as the antibiotic.53 E. coli was cultured in Miller's LB Broth with 50 μg/mL chloramphenicol and 100 μg/mL ampicillin. S. aureus was grown in 5 mL cultures in Tryptic Soy Broth without antibiotics. The cells were incubated at 37 °C on an orbital shaker (500 rpm) until an optical density (OD600) of 0.650.70 (M. smegmatis and S. aureus) or 0.330.40 (E. coli) at 600 nm, corresponding to a concentration of 13 108 CFU/mL, was reached (CFU = colony forming units from a single bacterial cell). Incubation of Cells with Photosensitizer. The 5 mL culture with a concentration of 13 108 CFU/mL was pelleted by centrifugation (10 min, 3716g) at room temperature, the supernatant discarded, and the cells were resuspended in a total volume of 5 mL of PBS
(phosphate buffered saline = 170 mM NaCl, 3.4 mM KCl, 10 mM Na2HPO4, 1.8 mM KH2PO4, pH 7.2 with additional 0.05% Tween 80) and the appropriate volume of the photosensitizer stock solution. The cells were incubated between 5 and 60 min in the dark and agitated by a vortex mixer set to the lowest speed. No degradation of CNC-Por (5) was observed in PBS solution over the time range examined in this study. Cell Illumination Conditions. All photosensitization experiments were performed using a noncoherent light source, PDT light model LC122 (LumaCare, U.S.A.), and the fluence rate was measured with an Orion power meter (Orphir Optronics Ltd., Israel). Aliquots (1 mL) of the cell suspension in PBS were added to a sterile 24-well plate (BD Falcon, flat bottom) and illuminated with visible light (400700 nm) with a fluence rate of 60 mW/cm2 for the duration of 15 or 30 min (corresponding to fluences of 54 or 108 J/cm2) while magnetically stirred. Tween-80 (0.05%) was added to the buffer to prevent excessive aggregation of the PS during the illumination process. After illumination, an aliquot was used for viability assays. All experiments were conducted in triplicate at a minimum. Cell Survival Assays. A total of 40 μL from the illuminated cell suspension was 1:10 serially diluted six times and plated on square plates (Middlebrook 7H10-ADS solid media for M. smegmatis, Miller's LB BrothAgar plates for E. coli and Tryptic Soy BrothAgar plates for S. aureus), as described by Jett and co-workers.54 The plates were incubated at 37 °C in the dark for 4860 h (M. smegmatis) or overnight (E. coli and S. aureus). The survival rate was determined from the ratio of CFU/mL of the illuminated solution and the dark control. Due to the plating technique employed, a maximum of a six log unit change in CFU/mL corresponding to g100 CFU/mL could be detected for an initial concentration of 1 108 CFU/mL. Survival rates of 95% of the available surface methylhydroxy groups. Appendage of the porphyrin onto the cellulose nanocrystalline surface was achieved by the Cu(I)-catalyzed HuisgenMeldal Sharpless 1,3-dipolar cycloaddition reaction.35,42,45,60,61 Several conditions, including temperature (room temperature to 60 °C), solvents (EtOH, DMF), and Cu catalysts (CuI, CuBr2/ascorbate,
[Cu(OTf)]2 3 tol), were surveyed, and CuBr2 in combination with ascorbate in DMF at elevated temperature in the presence of triethylamine proved to give the most optimal results. The choice of DMF as the solvent was based upon the solubility of the porphyrin 4. Puriﬁcation of the resulting product, an insoluble green crystalline material [(5), Scheme 1], was achieved by careful washing and centrifugation to remove both unreacted 4 and copper catalyst per literature precedent.62,63 IR Characterization of CNC-Por (5). Clear evidence for the successful reaction of the ethyne functional group in 4 with the azide containing cellulose nanocrystals 3 was obtained from IR spectroscopic analysis (Figure 1). The IR spectrum of the azide surface-modified cellulose, CNC-N3 (3; black trace), clearly exhibited an azide band at 2113 cm1, which is within the range of 21602080 cm1 expected for the antisymmetric azide stretching motion.64 Upon reaction with the ethyne containing porphyrin 4, the azide band in the IR spectrum of the resulting product 5 was diminished by 72%. Additionally, an intensity increase of the bands in the region around 1651 cm1 indicated the presence of CdN double bonds arising from the porphyrin and triazole linkage. The broad band centered around 1647 cm1 in the spectrum for the CNC-N3 (3) is most likely due to the bending motion of adsorbed water and overlaps with the CdN stretching modes for CNC-Por (5).65 Molecular Weight Determination and Porphyrin Loading of CNC-Por (5). The molecular weight gain attributable to the appended porphyrins was assessed by gel permeation chromatography (GPC). Due to the insolubility of cellulosic samples in organic solvents, the hydroxyl groups were benzoylated prior to GPC analysis. Samples of 3 and 5 were dissolved in the ionic liquid 1-allyl-3-methylimidazolium chloride and treated with benzoyl chloride. The weight average molecular weight (Mw), number average molecular weight (Mn), and consequently the distribution of molecular weight also known as polydispersity (Mw/Mn) were calculated from the GPC data. The molecular weight distribution of 5 clearly shifted to higher molecular weights with 102000 g/mol representing the weight average molecular weight (Mw) compared to 69000 g/mol (Mw) for 3 (Figure 2, Table 1). This 48% increase in the Mw further supports the notion of a covalent appendage between the porphyrin 4 and CNC-N3 (3). Further, we have attributed the increase in polydispersity (Mw/Mn) of the benzoylated CNC-Por sample when compared to that of the benzoylated CNC-N3 material, to a distribution of surface-bound porphyrins arising from the partial 3532
dx.doi.org/10.1021/bm200718s |Biomacromolecules 2011, 12, 3528–3539
Table 1. Molecular Weight Distributions of Benzoylated Derivatives of CNC-N3 (3) and CNC-Por (5) in THF
(Mw) 103 g/mol
(Mn) 103 g/mol
benzoylated CNC-Por (5), benzoylated
reaction of 4 with 3 (Table 1). From the molecular weight increase between CNC-N3 (3) and CNC-Por (5) and considering the average formula mass of the anhydrous glucose-N3 unit of 166 g/mol, we were able to estimate the porphyrin loading of the CNCs as one porphyrin molecule per 15 glucose molecules. Considering the degree of substitution of DS = 0.14 for the azide groups on the crystal surface, we estimate that approximately 50% of the azide groups were reacted with the cationic porphyrin, corresponding to an overall degree of substitution of DS = 0.07 for the porphyrin. Alternatively, the porphyrin loading was determined indirectly by measuring the Zn-ion content by atomic absorption spectroscopy of a CNC-Por (5) sample in 1 M HCl using the standard addition method.66 Under the assumption that one Zn-ion detected corresponds to one porphyrin molecule covalently attached to the cellulose nanocrystalline surface, a maximum loading of ∼0.16 ( 0.03 μmol porphyrin/mg 5 was obtained. Using this method, the porphyrin loading was determined as 1 porphyrin per ∼20 glucose units. Pulsed Field Gradient Spin Echo 1H NMR Spectroscopy. NMR spectroscopic characterization of CNC-Por (5) proved to be possible only upon acetylation due to the insolubility of this crystalline material in common solvents. Briefly, CNC-Por (5) was dissolved in 1-allyl-3-methylimidazolium chloride (AMIM-Cl) at 80 °C over 12 h and, subsequently, reacted with acetic anhydride. The resulting acetylated CNC-Por was rendered soluble in DMSO and, therefore, was amenable for characterization by NMR spectroscopy. The 1H NMR spectrum of acetylated 5 revealed the presence of proton resonances for cellulose along side with those of the porphyrin component. However, relative to the cellulose, the small concentration of the porphyrin (approximately 1 molecule/1520 glucose units), which had only been appended to the surface of the cellulose nanocrystals, did not allow for any further conclusions regarding the covalent conjugation between the two entities. Therefore, pulsed field gradient spin echo 1H NMR experiments (PFGSE-LED pulse sequence) were performed.49,52,67 The PFGSE-NMR technique allows for the determination of diffusion coefficients even for mixtures of compounds.68 Diffusion NMR, with its ability to draw conclusions about molecular size, shape, aggregation, or binding in complex solutions, has proven useful in a range of different fields such as bioanalytical, pharmaceutical, environmental, and materials chemistry.6974 In pulsed field gradient experiments, a magnetic gradient pulse whose strength varies throughout the sample is applied in addition to the static magnetic field. Thereby, it is possible to label the spins according to their translational position in the NMR tube. After this encoding pulse, the molecules are allowed to diffuse for a specified time period, after which a decoding gradient pulse is applied. If diffusion to a different part of the sample has occurred,
the decoding pulse will not completely reverse the phase change of the encoding pulse, and an attenuation of the NMR signal is observed. The change in resonance intensity for simple PFG pulse sequences is proportional to the diffusion coefficient (D) and square of the gradient pulse amplitude (G), as described in eq 1: I ¼ I0 exp½ DðGδγÞ2 ðΔ δ=3Þ
in which I0 denotes the signal intensity in the absence of a gradient pulse, δ the gradient duration, γ the magnetogyric ratio of the nucleus under investigation, and Δ the settling time. A plot of ln(I/I0) over G2 allows determination of D from the slope.75 Figure 3A shows the results of the pulsed ﬁeld gradient spin echo 1H NMR experiments with the acetylated compound 5. The aromatic resonances of the porphyrin moiety were found from 8.0 to 9.5 ppm, whereas those from the methyl groups of the N-methylpyridinium substituents showed a signal at 4.7 ppm. The proton signals for the acetylated cellulose backbone appeared at ∼2 ppm (acetyl groups) and between 3.5 and 5.2 ppm (cellulose backbone). A small attenuation of the signal intensity for the cellulose backbone of 5 was observed by increasing the gradient strength incrementally. Magniﬁcation of the aromatic porphyrin region around 89 ppm also exhibited an equally small change in signal intensity (Figures 3A and SD3). This indicated that both the porphyrin and the acetylated cellulose diﬀused at the same rate (estimated diﬀusion coeﬃcient D = 2 107 cm2/s, Table 2) and, therefore, strongly suggested that they were covalently connected. As a control experiment, Figure 3B shows the results for the PFGSE-1H NMR spectroscopic studies of a mixture of the porphyrin 4 and acetylated CNC-N3 (3). A faster loss in signal intensity for the porphyrin protons (i.e., δ 9.4 or 4.7 ppm as representative resonances, Figure SD3) when compared to the methyl groups of the acetylated CNC-N3 (3; δ 2.0 ppm) was noted. The respective diﬀusion coeﬃcients estimated from the NMR data diﬀer by an order of magnitude, with 2 106 cm2/s for the porphyrin 4 and 3 107 cm2/s for the acetylated CNC-N3, whereas the diﬀusion rates for acetylated CNC-Por and CNC-N3 were very similar (Table 2). Taken together, the results of the PFGSE-1H NMR spectroscopic studies strongly suggest the presence of a covalent bond, and not adventitious binding, between the porphyrin macrocycle and the cellulose nanocrystal in CNCPor (5). Thermogravimetric Analysis of CNC-Por (5). In our efforts to further confirm and elucidate the physicochemical characteristics of these novel materials, we also investigated the thermal behavior of the starting materials, porphyrin 4 and CNC-N3 (3) versus that of CNC-Por (5) by thermogravimetric analysis (Figure 4). The 5% weight losses for both porphyrin 4 and CNC-N3 (3) were observed at 235 and 285 °C, respectively. For CNC-Por (5), a different thermal gravimetric behavior was apparent. Two degradation profiles were observed, with minor degradation commencing around 210 °C (weight loss of 20%) and major decomposition above 320 °C. This difference in thermal behavior further supports our claim that the CNC-N3 (3) had been chemically modified upon a coupling reaction with the porphyrin 4, producing a covalent linkage between the two. Photodynamic Inactivation Studies with CNC-Por (5). The ability of CNC-Por (5) to inactivate E. coli, M. smegmatis, and S. aureus was evaluated. The bacteria were grown to a concentration of ∼108 colony forming units per mL (CFU/mL), resuspended in PBS-0.05% Tween-80 containing buffer, incubated with the 3533
dx.doi.org/10.1021/bm200718s |Biomacromolecules 2011, 12, 3528–3539
Figure 3. Pulsed ﬁeld gradient spin echo 1H NMR in DMSO-d6 of (A) acetylated CNC-Por, and (B) control experiments with a mixture of porphyrin 4 and acetylated CNC-N3. The indicated signals were used for the estimation of diﬀusion coeﬃcients.
Table 2. Estimated Diﬀusion Coeﬃcients (D) Determined from PFGSE-1H NMR Spectroscopy compound
CNC-Por (5, acetylated)
CNC-N3 (3, acetylated) mixture with porphyrin 4
photosensitizer in the dark (incubation time was varied from 5 to 60 min) and subsequently illuminated with white light (400700 nm) with a fluence rate of 60 mW/cm2 for 15 or 30 min (equivalent to a fluence of 54 or 108 J/cm2). The stock solution for 5 was prepared based on the porphyrin loading determined by atomic absorption spectroscopy, and concentrations listed hereafter refer to the concentration of porphyrin on 5 present in the suspension. The concentration dependence of the CNC-Por (5) photosensitizer for S. aureus and M. smegmatis at fixed incubation (30 min) and illumination times (15 min) is illustrated in Figure SD4, and suggested a 20 μM concentration of the PS for these studies. Control experiments included monitoring of cell survival in PBS buffered solution in the dark, PS treatment of the bacteria in the dark, and light exposure of bacterial suspensions to azide surface-modified cellulose (Table SD1). The percentage of survival was determined by the ratio of the colony count from illuminated and nonilluminated control cell suspensions.
Figure 4. Thermal gravimetric analysis of CNC-Por (5).
The results for light-treated samples as well as dark controls are shown in Figure 5. Of the three bacteria examined, the Gramnegative E. coli appeared to be the least susceptible to photodynamic inactivation by CNC-Por (5) at a porphyrin concentration of 20 μM (Figure 5A). No statistically signiﬁcant inactivation of E. coli was observed with 15 min illumination time under all incubation periods tested (P > 0.2). With longer illumination times (30 min) a 12 log unit reduction in the cell count was observable (P = 0.05 for 45 and 60 min incubation time). The dark incubation time before the illumination step did not appear to play 3534
dx.doi.org/10.1021/bm200718s |Biomacromolecules 2011, 12, 3528–3539
Figure 5. Photodynamic inactivation of (A) E. coli, (B) M. smegmatis, and (C) S. aureus using 20 μM CNC-Por (5) as the photosensitizer. The dark incubation time was varied over 5, 15, 30, 45, and 60 min. Displayed is the % survival in PBS buﬀered bacterial suspensions (black rectangle), CNC-Por dark control (navy blue rectangle) and light-treated samples after illumination times of 15 (sky blue rectangle) or 30 (light blue rectangle) min (total ﬂuences of 54 and 108 J/cm2, respectively, at 60 mW/cm2). As the plating technique employed to determine % survival did not allow for detection of survival rates of 3 log units of inactivation (30 min illumination) if CNC-Por (5) indeed was contaminated with 50100 nM of 4, but photodynamic inactivation with 20 μM 5 was e2 log units. Consequently, we conclude that levels of unbound porphyrin contamination must be well below 50 nM, and the porphyrin species detected in the supernatant was most likely due to small crystals of 5 that did not separate under the centrifugation conditions used. S. aureus was extremely sensitive to photodynamic inactivation with 4. Even at 10 nM of 4, a viable cell loss of 3 log units (15 min illumination) was observed. In this case, we cannot conclusively exclude the possibility that